Tunable Shape Memory Polymers from خ±-Amino Acid-Based Poly ... Shape memory polymers (SMPs)...
Embed Size (px)
Transcript of Tunable Shape Memory Polymers from خ±-Amino Acid-Based Poly ... Shape memory polymers (SMPs)...
Tunable Shape Memory Polymers from α‑Amino Acid-Based Poly(ester urea)s Gregory I. Peterson, Erin P. Childers, Hao Li, Andrey V. Dobrynin, and Matthew L. Becker*
Department of Polymer Science, The University of Akron, Akron, Ohio 44325-3909, United States
*S Supporting Information
ABSTRACT: The thermal shape memory behavior of poly(ester urea)s (PEUs) composed of varying α-amino acids and linear diols has been explored. The thermal, mechanical, and shape memory properties of PEUs are shown to be controlled by changing the amino acid and diol components of the polymer, without negatively affecting the shape memory performance of the polymer in most cases. These materials display triple-shape memory behavior and temperature memory properties due to a broad glass transition temperature interval. The versatility of the shape memory behavior of PEUs was explored by demonstrating shape transformations of thin films, salt leached scaffolds, and larger constructs. Overall good shape memory behavior in combination with the tunable properties of PEU materials makes them prime candidates for use as shape memory materials in biomedical applications.
■ INTRODUCTION Shape memory polymers (SMPs) provide materials that can change shape upon application of a stimulus and have shown considerable promise for use in biomedical applications.1−6
Self-tightening sutures,7 deployable structures in medical devices,8 shape changing scaffolds and surfaces,9,10 and drug delivery systems11 represent some of the potential uses of SMPs. The advantages of using polymers, as opposed to shape memory alloys,12,13 include the potential for biodegradability, lower cost, larger achievable strains during shape actuation, and tunable material properties. Considering the broad range of tissue types and corresponding mechanical properties encoun- tered in the body, the ability to tune a material’s properties to meet the demands of a particular application is vital. The simplest SMPs are dual-shape memory materials that
require, first, programming a temporary shape, followed by application of an appropriate stimulus (heat being the most common) to trigger recovery of the permanent shape.14−18
Other stimuli can be used such as light, chemical impetus, or various methods of indirect heating (e.g., photo-, electro-, and magneto-thermal transduction). The two basic requirements for a thermal SMP are possessing: 1) a reversible thermal transition (i.e., glass or melt transition) to activate and suppress chain mobility and 2) a cross-linked structure to prevent chain slippage and set the permanent shape.18 In addition, important design considerations for SMPs in biomedical applications include biodegradability, biocompatibility, compatible mechan- ical properties, and sterilizability.3 A wide range of thermal SMPs, including polyesters, polyurethanes, and polyacrylates, have been identified as viable candidates for biomedical applications,1,4,5,19,20 although the extent to which these materials meet the design considerations lacks a comprehensive study.
α-Amino acid-based poly(ester urea)s (PEUs) have recently emerged as an important class of tunable materials for biomedical applications. These materials are biodegradable, sterilizable, nontoxic, have nontoxic degradation products, and lead to no inflammatory response during degradation in vivo.21
Their mechanical properties can be tuned for use in both hard and soft tissues, such as bone and blood vessels.22−24
Additionally, the materials can be prepared with various functionalities for specific applications, such as peptides for bone growth,25 iodine for radiopacity,26 catechols for adhesion,27 fluorescent probes for visualization,28 and ther- apeutics for drug delivery.29 The main advantages of PEUs over many other biodegradable polymers include simple scalable synthesis, tunable degradation and mechanical properties, and mechanical properties derived from hydrogen bonding rather than crystallinity. This versatility, and the previously demon- strated examples of biocompatibility, makes PEUs viable candidates for a wide range of biomedical applications. We recently demonstrated that L-valine (VAL)-based PEUs
exhibit thermal shape memory behavior that takes advantage of a broad glass transition temperature (Tg), above which significant chain mobility could be activated, and shape programming and recovery were achieved.30 The materials do not have chemical cross-links but possess a strong hydrogen bonding network that form the physical cross-links required for shape imprinting. Excellent dual- and triple-shape memory performance was observed, and quadruple-shape memory behavior could be achieved by blending VAL-based PEUs with different diol chain lengths incorporated into the polymer
Received: April 1, 2017 Revised: May 9, 2017 Published: May 18, 2017
© 2017 American Chemical Society 4300 DOI: 10.1021/acs.macromol.7b00680 Macromolecules 2017, 50, 4300−4308
backbone. In this article, we explore the effect of amino acid and diol lengths on the shape memory behavior of PEUs prepared from L-alanine (ALA), L-isoleucine (ILE), L-phenyl- alanine (PHE), and the unnatural amino acid L-2-aminobutyric acid (ABA).
■ EXPERIMENTAL SECTION Materials. Chloroform was either obtained from an Inert Pure Solv
solvent purification system or dried over calcium hydride overnight and then distilled. All other reagents and solvents were used as obtained from commercial sources. Characterization. NMR spectra were collected with Varian NMR
spectrometers (300 and 500 MHz). All chemical shifts were reported in ppm (δ) and referenced to the chemical shifts of the residual solvent resonances (1H NMR, dimethyl sulfoxide (DMSO)-d6: 2.50 ppm;
13C NMR DMSO-d6: 39.50 ppm). The following abbreviations were used to explain the multiplicities: s = singlet, d = doublet, t = triplet, q = quartet, and m = multiplet. Number-average molecular mass (Mn) and postprecipitation molecular mass distribution (ĐM) were determined by size exclusion chromatography (SEC), and molecular mass values were determined relative to polystyrene standards. The SEC analyses were performed using a TOSOH HLC-8320 gel permeation chromatograph instrument with dimethylformamide (DMF) (con- taining 0.01 M LiBr) as eluent (flow rate of 1 mL/min and temperature of 50 °C) and a refractive index detector. The Tg of polymers was determined by differential scanning calorimetry (DSC, TA Q2000, scan rate of 20 °C/min) or dynamic mechanical analysis (DMA, TA Q800, 3 °C/min and a frequency of 1 Hz). X-ray diffraction (XRD) data were collected on a Rigaku Ultima IV X-ray diffractometer. IR spectra of monomers and polymers were collected on a Nicolet i550 FT-IR (Thermo Scientific) after dissolution in chloroform and application to a KBr salt plate (32 scans, 8 cm−1
resolution). Synthesis of VAL- and PHE-Based PEUs. The VAL- and PHE-
based PEUs were prepared and characterized as previously described.22,24
General Procedure for Synthesis of PEU Monomers. Either 1,6-hexanediol, 1,8-octanediol, 1,10-decanediol, or 1,12-dodecandiol (1.0 mol equiv), a L-amino acid (2.3 mol equiv), p-toluenesulfonic acid monohydrate (TsOH) (2.4 mol equiv), and toluene (1 mL per gram of TsOH) were added to round-bottom flask equipped with Dean− Stark trap and condenser. The solution was heated to reflux (ca. 110 °C) while stirring with a magnetic stir bar. After ca. 20 h, the reaction mixture was cooled to ambient temperature. The resulting precipitate was collected by vacuum filtration. The solid product was dissolved in minimal hot water and decolored using a small amount of activated carbon black for 2−3 min. This solution was filtered to remove the carbon black and was left to cool to room temperature. The precipitate was then recrystallized three times using hot water to give the purified monomer. Synthesis of m(1-ALA-6). The monomer was prepared by
following the general procedure described above, with the exception of the recrystallization procedure. The monomer was recrystallized four times from a 1:1 mixture (by volume) of ethanol and isopropanol. The monomer was prepared on a 145 mmol scale (based on the diol) and obtained with a 79% yield. 1H NMR (500 MHz, DMSO-d6, δ): 8.27 (s, 6H; NH3), 7.49 (d, J = 8.0 Hz, 4H; Ar−H), 7.12 (d, J = 7.8 Hz, 4H; Ar−H), 4.16 (m, 4H; CH2), 4.10 (q, J = 7.2 Hz, 2H; CH), 2.29 (s, 6H; CH3), 1.61 (m, 4H; CH2), 1.39 (d, J = 7.2 Hz, 6H; CH3), 1.35 (m, 4H; CH2).
13C NMR (126 MHz, DMSO-d6, δ): 169.92, 145.21, 137.89, 128.10, 125.46, 65.49, 47.93, 27.76, 24.71, 20.75, 15.70. IR (cm−1): 1743 (−C−(CO)−O−). Synthesis of m(1-ALA-8). The monomer was prepared by
following the general procedure described above, with the exception of the recrystallization procedure. The monomer was recrystallized four times from a 1:1 mixture (by volume) of ethanol and isopropanol. The monomer was prepared on a 147 mmol scale (based on the diol) and obtained with a 79% yield. 1H NMR (500 MHz, DMSO-d6, δ): 8.27 (s, 6H; NH3), 7.49 (d, J = 8.0 Hz, 4H; Ar−H), 7.12 (d, J = 7.8
Hz, 4H; Ar−H), 4.13 (m, 6H; CH2 and CH), 2.29 (s, 6H; CH3), 1.59 (m, 4H; CH2), 1.39 (d, J = 7.2 Hz, 6H; CH3), 1.32 (m, 8H; CH2).
13C NMR (126 MHz, DMSO-d6, δ): 169.92, 145.27, 137.83, 128.10, 125.45, 65.56, 47.92, 28.43, 27.87, 25.05, 20.71, 15.69. IR (cm−1): 1749 (−C−(CO)−O−).
Synthesis of m(1-ALA-10). The monomer was prepared by following the general procedure described above, with the exception of the recrystallization procedure. The monomer was recrystallized four times from a 1:1 mixture (by volume